SRIM simulation results for 40 keV ion implantation into PMMA (
The recent results obtained on the ion-irradiation-induced carbon nanostructures in optoelectronic polymer materials exemplified by boron-ion-implanted polymethylmethacrylate (B:PMMA) with an energy of 40 keV, ion doses from 6.25 × 1014 to 5.0 × 1016 ions/cm2, and current density <2 μA/cm2 are reviewed. The positron annihilation spectroscopy (slow positron beam spectroscopy based on Doppler broadening of positron annihilation gamma rays as a function of incident positron energy and positron annihilation lifetime at a positron energy of 2.15 keV, and temperature-dependent positron annihilation lifetime spectroscopy), optical UV-visible spectroscopy, Raman spectroscopy, electrical (current–voltage) measurements, and nanoindentation test are chosen as the main experimental tools for the investigation of low-energy ion-induced processes in B:PMMA. The formation of carbon nanostructures is confirmed for the samples irradiated with higher ion fluences (>1016 ions/cm2) and the experimental results of the comprehensive study are found to be in a good agreement with SRIM (stopping and range of ions in matter) simulation results.
- ion irradiation
- optoelectronic materials
- boron-ion-implanted polymethylmethacrylate
- carbon nanostructures
Ion implantation is a powerful experimental approach for structural modification of materials. In case of organic media, the interest to ion-irradiated polymers is due to the ion implantation being one of the effective technological methods to turn dielectric polymers into semiconductors  as well as to improve surface-sensitive mechanical properties of polymers for hard-materials applications . Substantial improvements in hardness, wear resistance, oxidation resistance, resistance to chemicals, and electrical conductivity are the main characteristics attained by polymeric materials after their low-to-medium-energy ion implantation [3–7].
The formation of free radicals at lower ion doses (<1016 ions/cm2) and carbonization at higher ion doses (>1016 ions/cm2) in the most polymeric materials are of general concept [8–10]. In particular, the ion irradiation of polymers leads to the scission and cross-linking of polymer chains, formation of volatile low-molecular fragments, and carbonization of the implanted layer. The carbonization process depends strongly on the implantation dose or/ and ion current density. As ion dose increases, the several stages can be distinguished for carbonization to be occurred. The formation of pre-carbon structures, nucleation, and growth of the carbon-enriched clusters, aggregation of the clusters, formation of network of conjugated bonds, and transition to amorphous carbon or graphite-like material are the main stages predicted in literature [8–10]. Despite numerical studies of carbonization processes in polymers, the problem remains to understand better how the carbonaceous phase or carbon nanostructures formed under high-dose ion implantation could be dependent on the type of polymer matrix. In this respect, a lot of efforts have been made by researchers studying the B+-ion implantation into various polymer matrix such as polycarbonate, Kapton, polyethylene, polyamide, polyimide, poly(ethylene terephthalate), cellulose, polypropylene, polystyrene, polyethersulfone, and others ([2, 4, 5, 11–25] and references therein). At the same time, the B+-ion implantation into widely used in practice polymer polymethylmethacrylate (PMMA) was not studied so far.
The interest to B+-ion implantation of polymers is due to formation of buried carbonaceous layer leading to increasing conductivity [20, 23]. Also, B+-ion implantation into polymeric matrix results in significant increase of surface-sensitive mechanical properties. So, Lee et al.  reported the ion-induced improvement in hardness of Kapton irradiated by three different ion species, He, B, and Si at 200 keV to a dose of 3.5 × 1019 ions/m2, where boron produced the largest improvement in hardness among the three, not following the increasing trend in atomic number.
The selection of PMMA matrix to be used for B+-ion implantation is due to an importance of this polymer for construction of many optical components (waveguides, lenses, prisms, etc.), lithography, biomedical applications, etc. ([26–30] and references therein). PMMA was also a subject for implantation with Ag+-ions [9, 31] to fabricate composite structures with silver nanoparticles for plasmonic applications as well as for implantation with C+, N+ and Ar+-ions [29, 30] that may find an extensive application in fabrication of various optoelectronic devices including organic light-emitting diodes, backlight components in liquid crystal display systems, diffractive elements, solar cells, waveguides, microcomponents for integrated optical circuits, etc. The well-known key performance and important characteristics of PMMA such as a long-term stability in outdoor environments, excellent surface hardness, light weight, outstanding transmittance and optical clarity, optical design flexibility and control, etc. , and high stability upon positron irradiation at room temperature  are also taken into account at the selection of basic polymeric matrix for low-energy ion implantation.
In this chapter, a review of recent results obtained using proper experimental and simulation techniques on the boron-ion-implanted polymethylmethacrylate (B:PMMA) is presented. As a result, the formation of ion-irradiation-induced carbon nanostructures in optoelectronic polymer materials exemplified by B:PMMA is evidently confirmed.
2.1. Sample preparation and SRIM simulation
The B+-ion implantation with the energy of 40 keV, doses from 6.25 × 1014 to 5.0 × 1016 ions/cm2 and current density < 2 μA/cm2 into the optically transparent PMMA plates (1.2 mm thickness) was performed under a pressure of 10−5 Torr at room temperature by an “ILU-3” ion accelerator at the Kazan Physical-Technical Institute (KPTI, Russia) similar to as it was earlier done for Xe+ and Ag+ ions .
For comparative analysis of depth profiles of implanted ions and introduced vacancies in respect to ion mass, SRIM (stopping and range of ions in matter) simulations were carried out for 40 keV He+, B+, O+, P+, Cl+, Cu+, Ag+, Xe+, and Au+ ions implanted into PMMA using the free of charge software of version SRIM-2013 .
2.2. Positron annihilation spectroscopy measurements
Positron annihilation spectroscopy (PAS) measurements with slow positron beam spectroscopy (SPBS) based on Doppler broadening of positron annihilation gamma-rays as a function of incident positron energy and positron annihilation lifetime at constant positron energy were performed at the National Institute of Advanced Industrial Science and Technology (AIST, Japan) . Doppler broadening spectra (
PAS measurements with positron annihilation lifetime spectroscopy (PALS) and Doppler broadening of annihilation line (DBAL) techniques in the temperature range of 50–300 K using helium cryostat (Closed Cycle Refrigerator, Janis Research Company, Inc., USA) and vacuum equipment (Pfeiffer Vacuum, HiCUBE, Germany) were carried out at the Institute of Physics, Slovak Academy of Sciences (IPSAS, Slovakia) [37–39]. The samples were measured in the cycles of heating and cooling with step of 20 K and elapsed time of 4–5 hours per point. At the selected temperatures, the elapsed time was extended for better statistics in the lifetime spectra. For these temperatures, the continuous lifetime analysis technique to obtain the distributions of
2.3. Optical spectroscopy measurements
Optical UV-visible spectroscopy measurements were performed using a SHIMADZU-UV 3100PC spectrophotometer in the range of 200–800 nm at AIST, Japan .
2.4. Raman spectroscopy measurements
Room temperature Raman spectra were recorded using a Renishaw Raman inVia Reflex spectrometer in the 400–3800 cm−1 range with a spectral resolution of ≤1 cm−1 . The 514 nm Modu-Laser Stellar-REN Pro 514/50 Argon Laser and 785 nm Near Infrared Diode Laser lines were applied as the excitation source. In order to avoid heat-induced effects, the laser power was set at 10 mW. A standard calibration of wavenumber scale with Si plate was used. The Raman spectroscopy measurements were performed at The John Paul II Catholic University of Lublin (KUL, Poland).
2.5. Electrical measurements
The electrical measuring system was developed at the IPSAS (Slovak Republic) . The measurement of current vs. voltage (
2.6. Nanoindentation test
Nanoindentation test was carried out using an ultra nano hardness tester (UNHT) with a diamond Berkovich indenter at the Lublin University of Technology (LUT, Poland) [45, 46]. Advantages of the new UNHT design applied for nanoindentation test compared to the conventional nano indenter (or NHT) design, both developed by CSM Instruments (Switzerland) , allow us to make measurements with high performance. The UNHT experiment was done in a progressive multicycle mode. The details of the progressive multicycle mode parameters used are reported elsewhere .
3. Results and discussion
3.1. SRIM simulation data
Figure 1 shows the typical SRIM simulation results for B+-implantation into PMMA at energy of 40 keV [36, 45]. Numerical values of SRIM simulation for 40 keV He+, B+, O+, P+, Cl+, Cu+, Ag+, Xe+, and Au+ ions into PMMA are gathered in Table 1 .
The SRIM data, presented in Table 1, were used for estimation a predicted thickness of implanted layer . Let us to explain it on the example of the modified PMMA by 40 keV accelerated B+ ions. A mean penetration range (
3.2. Positron annihilation spectroscopy data
SPBS, often called variable-energy PAS, is a powerful experimental tool widely used for evaluation of defects in solids as a function of depth (defect depth profiling) by varying the positron energy in the range of a few eV to tens keV (for review, see Ref. ). Thus, SBPS could be a very effective for the detection of defects induced by ion implantation, which are localized near the surface of material. At first, the un-implanted PMMA and implanted B:PMMA were characterized by Doppler broadening of annihilation gamma rays (or DBAL) as a function of incident positron energy in the range of 0–30 keV. And then, using Doppler broadening results, the PAL spectra at incident positron energy of 2.15 keV were measured and analyzed for the investigated samples. Figure 2 shows the typical variable-energy DBAL and PAL results obtained, the explanation of which has been done in .
It should only be emphasized here that there are two different processes seen from the
Thus, the expected two processes of polymer structure modification upon low-energy ion implantation—formation of free radicals at lower fluences (< 1016 ions/cm2) and carbonization at higher fluences (>1016 ions/cm2)—are plausibly confirmed .
The results of temperature dependent PALS measurements of the investigated pristine PMMA and implanted B:PMMA samples at lower ion dose (3.13 × 1015 ions/cm2) and at higher ion dose (3.75 × 1016 ions/cm2) are demonstrated in Figure 3. The detail description and possible explanation of these data have been presented in . Two structural transitions in the vicinity of ~150 and ~250 K, ascribed to
The threshold temperatures nearby ~150 and ~250 K for PMMA are also detected on Doppler parameters
New results are also obtained from the PALS study of B:PMMA on the free-volume voids distribution at room temperature  as shown in Figure 5. Namely, estimating the distribution of
3.3. Optical spectroscopy data
Application of UV-visible optical absorption spectroscopy for investigation of ion-implanted polymeric materials has already been reported for the Ag+-implanted PMMA, ORMOCER, and Epoxy resin [31, 34, 56–59] as well as for the C+, N+, and Ar+-implanted PMMA [29, 30]. It has been suggested by the authors that ion irradiation creates compact carbonaceous clusters in polymers, which may also be responsible for a narrowing of optical band gap, enhanced electrical conductivity, and increasing optical absorbance (for example, see [31, 34, 56]). In the case of the investigated B:PMMA, it is found the gradual increase of absorbance at lower fluences (<1016 ions/cm2) and saturation of absorbance at higher fluences (>1016 ions/cm2) as shown in Figure 6 .
The observed increasing absorbance for the B:PMMA samples in the course of the ion implantation should be also interpreted as the signature on the formation of carbonaceous clusters which are plausibly confirmed by slow positrons .
3.4. Raman spectroscopy data
Figure 7 shows the Raman spectra of the investigated samples excited by 514 nm and 785 nm diode laser lines . Identification of the observed Raman bands has been reported in . The ion-irradiation-induced structural changes as revealed from Raman study can be summarized as follows. New C=C and C−C bands in the vicinity of ~1590 and 1322 cm−1, respectively, are formed for the as-implanted samples at higher fluences (>1016 ions/cm2). At the same time, the decreasing intensity of CH2 band at ~815 cm−1, C=O band at ~1730 cm-1, O−CH3 band at ~991 and 2845 cm-1, and C−H band at ~1455, 2955, and 3001 cm−1 is detected.
In particular, Raman spectroscopy data for excitation by the laser wavelength of 785 nm seem to be additional confirmation for the carbonization processes in the B:PMMA. Indeed, new Raman bands at ~1325 and 1590 cm-1, attributed to C−C and C=C vibrations, respectively, are detected only for the ion-irradiated samples with higher fluences (>1016 ions/cm2). These two new Raman bands may also be attributed to the so-called D and G peaks in the region of 1300-1600 cm−1 which are the main peaks characteristic for graphite and graphene structure [60–66]. The intensity ratio of the D and G peaks
A correlation between slow positron beam and Raman spectroscopy results for B:PMMA is mentioned in our recent works . Table 2 gives the SPBS data, exemplified by
|6.25 × 1014||1.752||34.6||No peaks|
|3.13 × 1015||1.752||34.8||No peaks|
|2.5 × 1016||No
|5.0 × 1016||No
3.5. Electrical measurements data
The un-implanted PMMA and as-implanted B:PMMA samples were measured at 300 K and 360 K with DC method . It was supposed that the conductive layer in ion-implanted polymer is dependent on the temperature and at a higher temperature the effect of increasing conductivity with temperature will be more pronounced. In order to avoid a possible structural change in polymer matrix, the maximum temperature at 360 K was selected in the electrical measurement experiment, not exceeding the glass transition temperature
Figure 8 shows the obtained
The numerical values of the
3.6. Nanoindentation test data
A first time the results of investigation of the influence of low dose (6.25 × 1014 ions/cm2) B+-ion-irradiation on the mechanical properties (hardness and elastic modulus) of PMMA probed by nanoindentation with UNHT in the range of 300–1100 nm indentation depth have been reported in . It has been established that the hardness and elastic modulus versus maximum indentation depth illustrate the main difference between the un-implanted (pristine) and ion-implanted samples in the range up to about 400 nm. The same value of the maximum penetration depth of B+-ions into PMMA has been found using SPBS and SRIM simulation . As a continuation of the nanoindentation test of the B:PMMA, the averaged values of indentation hardness versus maximum indentation depth for the un-implanted and as-implanted samples with ion doses of 6.25 × 1014, 1.25 × 1016, 2.5 × 1016, and 3.75 × 1016 ions/cm2 are plotted in Figure 9 .
One may see that the hardness dependence on the maximum indentation depth demonstrates the difference between the PMMA and B:PMMA samples in the entire range studied up to 1100 nm with the largest changes in the vicinity of 300-400 nm in consistence with the maximum penetration depth of B+-ions into PMMA as revealed from SPBS measurements and SRIM simulation . The observed improving of surface-sensitive mechanical properties of B:PMMA by ion beam processing is obviously detected to be more significant as ion dose increases, that may be suitable for hard-materials applications. According to Lee et al.  these properties are apparently related to the effectiveness of cross-linking. Besides, the abovementioned formation of carbon nanostructures upon high-dose ion implantation (>1016 ions/cm2) seems to be also important. But further increase of hardness with deeper penetration of indenter up to 1100 nm for higher fluences (3.75 × 1016 B+/cm2) was found to be very interesting and not fully understood yet (see Figure 9). Actually, similar results that the hardness of B+-implanted polycarbonate increased with increasing ion dose has also been observed in Ref.  but only for penetration of indenter up to 400 nm, that is not so far from the implanted layer as in our case. A deeper understanding the low-energy ion-irradiation-induced processes in polymeric materials exemplified by PMMA irradiated by accelerated light, middle, and heavy ions is still required.
The formation of carbon nanostructures has been confirmed for the B:PMMA samples irradiated with higher ion fluences (>1016 ions/cm2) and the experimental results of the comprehensive study have been found to be in a good agreement with SRIM simulation results. It is expected that the results obtained for low-energy B+-ion implantation into PMMA will have impact on research and development in the fields of nanoscience, nanotechnology, and nanooptoelectronics, in particular, to be potentially of interest for fabrication of organic luminescent devices, backlight components in liquid crystal display systems, diffractive elements and microcomponents for integrated optical circuits, solar cells, waveguides, etc. similarly as it has been foreseen for low-energy C+, N+, and Ar+-ion implantation into PMMA [29, 30].
T.S. Kavetskyy acknowledges the SAIA for scholarships in the Institute of Physics of SAS within the National Scholarship Program of the Slovak Republic. This work was also supported in part by the SFFR of Ukraine (Nos. F40.2/019 and F52.2/003) and MES of Ukraine (Nos. 0114U002616 and 0114U002617). A.L. Stepanov thanks the RFBR (No. 15-48-02525) and RSF (No. 14-13-00758) in Russia for financial support.
Wasserman B, Braunstein G, Dresselhaus MS, Wnek GE. Implantation-induced conductivity of polymers. Mater. Res. Soc. Symp. Proc. 1983; 27: 423–428. DOI: 10.1557/PROC-27-423
Lee EH, Rao GR, Mansur LK. Improved hardness and wear properties of B-ion implanted polycarbonate. J. Mater. Res. 1992; 7: 1900–1911. DOI: 10.1557/JMR.1992.1900
Bridwell LB. Ion implantation of polymers for electrical conductivity enhancement. Solid State Phenomena. 1992; 27: 163–180. DOI: 10.4028/www.scientific.net/SSP.27.163
Lee EH, Rao GR, Lewis MB, Mansur LK. Ion beam application for improved polymer surface properties. Nucl. Instr. Meth. B. 1993; 74: 326–330. DOI: 10.1016/0168-583X(93)95070-L
Rao GR, Lee EH, Mansur LK. Structure and dose effects on improved wear properties of ion-implanted polymers. Wear 1993; 162–164: 739–747. DOI: 10.1016/0043-1648(93)90074-V
Goyal PK, Kumar V, Gupta R, Kumar S, Kumar P, Kanjilal D. Effect of Ar+ ion implantation on electrical conductivity of polycarbonate. AIP Conf. Proc. 2011; 1349: 543–549. DOI: 10.1063/1.3605973
Goyal PK, Kumar V, Gupta R, Kumar S, Kumar P, Kanjilal D. Study of electrical conductivity of Kr+ ion implanted polycarbonate in relation to carbon structure. AIP Conf. Proc. 2011; 1393: 147–151. DOI: 10.1063/1.3653652
Sviridov DV. Chemical aspects of implantation of high-energy ions into polymeric materials. Russ. Chem. Rev. 2002; 71: 315–327. DOI: 10.1070/RC2002v071n04ABEH000710
Stepanov AL. Optical properties of metal nanoparticles synthesized in a polymer by ion implantation: A review. Tech. Phys. 2004; 49: 143–153. DOI: 10.1134/1.1648948
Popok VN. Ion implantation of polymers: Formation of nanoparticulate materials. Rev. Adv. Mater. Sci. 2012; 30: 1–26. http://www.ipme.ru/e-journals/RAMS/no_13012/01_popok.pdf
Fink D, Müller M, Stettner U, Behar M, Fichtner PFP, Zawislak FC, Koul S. Non-regular depth profiles of light ions implanted into organic polymer films. Nucl. Instr. Meth. B 1988; 32: 150–154. DOI: 10.1016/0168-583X(88)90199-1
Guimaraes RB, Amaral L, Behar M, Fichtner PFP, Zawislak FC, Fink D. Implanted boron depth profiles in the AZ111 photoresist. J. Appl. Phys. 1988; 63: 2083–2085. DOI: 10.1063/1.341112
Azarko II, Hnatowicz V, Kozlov IP, Kozlova EI, Odzhaev VB, Popok VN. EPR spectroscopy of ion implanted polymer films. Phys. Stat. Sol. A 1994; 146: K23–K27. DOI: 10.1002/pssa.2211460239
Azarko II, Karpovich IA, Kozlov IP, Kozlova EI, Odzhaev VB, Popok VN, Hnatowicz V. Influence of ion implantation on the properties of polymer films. Solid State Commun. 1995; 95: 49–51. DOI: 10.1016/0038-1098(95)00905-1
Odzhaev VB, Azarko II, Karpovich IA, Kozlov IP, Popok VN, Sviridov DV, Hnatowicz V, Jankovskij ON, Rybka V, Švorčík V. The properties of polyethylene and polyamide implanted with B+ ions to high doses. Mater. Letters 1995; 23: 163–166. DOI: 10.1016/0167-577X(94)00274-6
Popok VN, Odzhaev VB, Kozlov IP, Azarko II, Karpovich IA, Sviridov DV. Ion beam effects in polymer films: Structure evolution of the implanted layer. Nucl. Instr. Meth. B 1997; 129: 60–64. DOI: 10.1016/S0168-583X(97)00208-5
Vacik J, Cervena J, Fink D, Klett R, Hnatowicz V, Popok V, Odzhaev V. High fluence boron ion implantation into polymers. Radiat. Eff. Def. Solids. 1997; 143: 139–156. DOI: 10.1080/10420159708212955
Kozlov IP, Odzhaev VB, Karpovich IA, Popok VN, Sviridov DV. Optical properties of ion-implanted polymer layers. J. Appl. Spectr. 1998; 65: 390–394. DOI: 10.1007/BF02675458
Kozlov IV, Odzhaev VB, Popok VN, Azarko II, Kozlova EI. Paramagnetic properties of ion-implanted polymer layers. J. Appl. Spectr. 1998; 65: 583–588. DOI: 10.1007/BF02675652
Popok VN, Karpovich IA, Odzhaev VB, Sviridov DV. Structure evolution of implanted polymers: Buried conductive layer formation. Nucl. Instr. Meth. B. 1999; 148: 1106–1110. DOI: 10.1016/S0168-583X(98)00799-X
Vacík J, Hnatowicz V, ČervenáJ, Peřina V, Popok V, Odzhaev V, Fink D. High fluence boron implantation into polyimide. Nucl. Instr. Meth. B 1999; 148: 1126–1130. DOI: 10.1016/S0168-583X(98)00814-3
Vacík J, Hnatowicz V, ČervenáJ, Peřina V, Popok V, Odzhaev V, Švorčík V, Rybka V, Arenholz E, Fink D. Annealing behaviour of boron atoms implanted into polyethyleneterephtalate. Nucl. Instr. Meth. B 2000; 166–167: 637–640. DOI: 10.1016/S0168-583X(99)01049-6
Odzhaev VB, Popok VN, Kozlova EI, Jankovskij ON, Karpovich IA. Electrical properties of polyethylene modified by ion implantation and diffusion. Nucl. Instr. Meth. B 2000; 166–167: 655–659. DOI: 10.1016/S0168-583X(99)01212-4
Popok VN, Odzhaev VB, Azarko II, Kozlov IP, Sviridov DV, Hnatowicz V, Vacík J, ČervenáJ. Multistage ion implantation of polyamide-6 films. Nucl. Instr. Meth. B 2000; 166–167: 660–663. DOI: 10.1016/S0168-583X(99)01211-2
Popok VN, Azarko II, Odzhaev VB, Tóth A, Khaibullin RI. High fluence ion beam modification of polymer surfaces: EPR and XPS studies. Nucl. Instr. Meth. B 2001; 178: 305–310. DOI: 10.1016/S0168-583X(00)00491-2
Kuo SW, Kao HC, Chang FC. Thermal behavior and specific interactions in high glass transition temperature PMMA copolymer. Polymer 2003; 44: 6873–6882. DOI: 10.1016/j.polymer.2003.08.026
Teixeira FS, Salvadori MC, Cattani M, Brown IG. Gold-implanted shallow conducting layers in polymethylmethacrylate. J. Appl. Phys. 2009; 105: 064313-1–064313-5. DOI: 10.1063/1.3088874
Tsvetkova T, Balabanov S, Avramov L, Borisova E, Angelov I, Sinning S, Bischoff L. Photoluminescence enhancement in Si+ implanted PMMA. Vacuum 2009; 83: S252–S255. DOI: 10.1016/j.vacuum.2009.01.075
Wang J, Zhu F, Zhang B, Liu H, Jia G, Liu C. Photoluminescence and reflectivity of polymethylmethacrylate implanted by low-energy carbon ions at high fluences. Appl. Surf. Sci. 2012; 261: 653–658. DOI: 10.1016/j.apsusc.2012.08.076
Gupta R, Kumar V, Goyal PK, Kumar S. Optical characterization of poly(methyl methacrylate) implanted with low energy ions. Appl. Surf. Sci. 2012; 263: 334–338. DOI: 10.1016/j.apsusc.2012.09.056
Stepanov AL. Optical extinction of metal nanoparticles synthesized in polymer by ion implantation. In: Nicolais L, Carotenuto G, editors. Metal-Polymer Nanocomposites. Italy: Wiley; 2005. p. 241–263. DOI: 10.1002/0471695432.ch8
Colburn P. Acrylic materials in PV applications: Making an informed choice. Evonik Industries – NREL PV Reliability Workshop [Internet]; 2011. Available from: http://www1.eere.energy.gov/solar/pdfs/pvmrw2011_23_cpv_colburn.pdf [accessed 2011-02-17].
Qi N, Chen ZQ, Uedono A. Molecular motion and relaxation below glass transition temperature in poly (methyl methacrylate) studied by positron annihilation. Rad. Phys. Chem. 2015; 108: 81–86. DOI: 10.1016/j.radphyschem.2014.11.018
Stepanov AL, Abdullin SN, Petukhov VY, Osin YN, Khaibullin IB. Formation of metal-polymer composites by ion implantation. Phil. Mag. B 2000; 80: 23–28. DOI: 10.1080/13642810008218336
Ziegler JF, Biersak JP, Littmark U. The Stopping and Range of Ions in Solids. New York: Pergamon; 1996. http://www.srim.org/
Kavetskyy T, Tsmots V, Kinomura A, Kobayashi Y, Suzuki R, Mohamed HFM, Šauša O, Nuzhdin V, Valeev V, Stepanov AL. Structural defects and positronium formation in 40 ke V B+-implanted polymethylmethacrylate. J. Phys. Chem. B 2014; 118: 4194–4200. DOI: 10.1021/jp410763t
Kavetskyy TS, Tsmots VM, Voloshanska SY, Šauša O, Nuzhdin VI, Valeev VF, Osin YN, Stepanov AL. Low-temperature positron annihilation study of B+-ion implanted PMMA. Low Temp. Phys. 2014; 40: 747–751. DOI: 10.1063/1.4892646
Kavetskyy T, Tsmots V, Šauša O, Stepanov AL. Structural modification of chalcogenide glasses by gamma-irradiation studied with DBAL technique. Phys. Status Solidi C 2012; 9: 2420–2423. DOI: 10.1002/pssc.201200252
Kavetskyy TS, Tsmots VM, Voloshanska SY, Šauša O, Stepanov AL. Low-temperature Doppler broadening of annihilation line study of PMMA. In: Proceedings of the 6th International Scientific and Technical Conference on Sensor Electronics and Microsystem Technologies (SEMST-6); 29 September–3 October 2014; Astroprint; Odessa; 2014. p. 226.
Shukla A, Peter M, Hoffmann L. Analysis of positron lifetime spectra using quantified maximum entropy and a general linear filter. Nucl. Instr. Meth. A 1993; 335: 310–317. DOI: 10.1016/0168-9002(93)90286-Q
Kirkegaard P, Eldrup M, Mogensen OE, Pedersen NJ. Program system for analysing positron lifetime spectra and angular correlation curves. Comp. Phys. Commun. 1981; 23: 307–335. DOI: 10.1016/0010-4655(81)90006-0
Bandžuch P, MorháčM, Krištiak J. Study of the Van Cittert and gold iterative methods of deconvolution and their application in the deconvolution of experimental spectra of positron annihilation. Nucl. Instr. Meth. A 1997; 384: 506–515. DOI: 10.1016/S0168-9002(96)00874-1
Kavetskyy T, Nowak J, Borc J, Rusnák J, Šauša O, Stepanov AL. Carbonization in boron-ion-implanted polymethylmethacrylate as revealed from Raman spectroscopy and electrical measurements. Spectroscop Lett. 2016; 49: 5–10. DOI: 10.1080/00387010.2015.1044113
National Instruments [Internet]. 2014. Available from: http://www.ni.com/datasheet/pdf/en/ds-15 [accessed 2014-11-06].
Kavetskyy TS, Borc J, Kukhazh YY, Stepanov AL. The influence of low dose ion-irradiation on the mechanical properties of PMMA probed by nanoindentation. In: Petkov P, Tsiulyanu D, Kulisch W, Popov C, editors. Nanoscience Advances in CBRN Agents Detection, Information and Energy Security. NATO Science for Peace and Security Series – A: Chemistry and Biology. The Netherlands: Springer; 2015. p. 65–71. DOI: 10.1007/978-94-017-9697-2_7
Kavetskyy TS, Kukhazh YY, Borc J, Stepanov AL. Nanoindentation of boron-ion implanted polymethylmethacrylate up to 1100 nm indentation depth. In: Proceedings of the XXII International Conference on Ion-Surface Interactions (ISI-2015); 20–24 August 2015; NRNU MEPh I; Moscow; 2015. Vol. 2. p. 132–135.
Introduction on Instrumented Indentation [Internet]. 2013. Available from: http://www.csm-instruments.com [accessed 2013-11-15].
Kavetskyy TS, Stepanov AL. Spectroscopic investigations of ion-induced processes in polymethylmethacrylate at low-energy boron-ion implantation. In: Proceedings of the XXII International Conference on Ion-Surface Interactions (ISI-2015); 20–24 August 2015; NRNU MEPh I; Moscow; 2015. Vol. 3. p. 339–342.
Schultz PJ, Lynn KG. Interaction of positron beams with surfaces, thin films, and interfaces. Rev. Mod. Phys. 1988; 60: 701–779. DOI: 10.1103/Rev Mod Phys.60.701
Kobayashi Y, Ito K, Oka T, He C, Mohamed HFM, Suzuki R, Ohdaira T. Application of positron beams to the study of positronium-forming solids. Appl. Surf. Sci. 2008; 255: 174–178. DOI: 10.1016/j.apsusc.2008.05.278
Krištiak J, Krištiakova K, Šauša O. Phase transition in C60 observed by positron annihilation. Phys. Rev. B. 1994; 50: 2792–2794. DOI: 10.1103/Phys Rev B.50.2792
Liao KS, Fu YJ, Hu CC, Chen JT, Lin DW, Lee KR, Tung KL, Jean YC, Lai JY. Microstructure of carbon molecular sieve membranes and their application to separation of aqueous bioethanol. Carbon 2012; 50: 4220–4227. DOI: 10.1016/j.carbon.2012.05.003
Wang CL, Hirade T, Maurer FHJ, Eldrup M, Pedersen NJ. Free-volume distribution and positronium formation in amorphous polymers: Temperature and positron-irradiation-time dependence. J. Chem. Phys. 1998; 108: 4654–4661. DOI: 10.1063/1.475876
Pujari PK, Tashiro M, Tseng CY, Honda Y, Nishijima S, Tagawa S. Low-temperature positron studies in polymethylmethacrylate. Mater. Sci. Forum 2001; 363–365: 275–277. DOI: 10.4028/www.scientific.net/MSF.363-365.275
He CQ, Dai YQ, Wang B, Wang SJ. Molecular weight effect on the microstructure and local motion in high molecular weight polymer observed by positrons. Mater. Sci. Forum 2001; 363–365: 309–312. DOI: 10.4028/www.scientific.net/MSF.363-365.309
Stepanov AL. Nanofillers: Synthesis of metal nanoparticles in viscous polymer. In: Nicolais L, Borzacchiello A, editors. Wiley Encyclopedia of Composites. 2nd ed. Italy: Wiley; 2012. p. 1–9. DOI: 10.1002/9781118097298.weoc157
Stepanov AL, Kiyan R, Ovsianikov A, Nuzhdin VI, Valeev VF, Osin YN, Chichkov BN. Synthesis and optical properties of silver nanoparticles in ORMOCER. Appl. Phys. A 2012; 108: 375–378. DOI: 10.1007/s00339-012-6894-6
Stepanov AL. Synthesis of silver nanoparticles in dielectric matrix by ion implantation: A review. Rev. Adv. Mater. Sci. 2010; 26: 1–29. http://www.ipme.ru/e-journals/RAMS/no_12610/stepanov.pdf
Takele H, Greve H, Pochstein C, Zaporojtchenko V, Faupel F. Plasmonic properties of Ag nanoclusters in various polymer matrices. Nanotechnology 2006; 17: 3499–3505. DOI: 10.1088/0957-4484/17/14/023
Tuinstra F, Koenig JL. Raman spectrum of graphite. J. Chem. Phys. 1970; 53: 1126–1130. DOI: 10.1063/1.1674108
Elman BS, Dresselhaus MS, Dresselhaus G, Maby EW, Mazurek H. Raman scattering from ion-implanted graphite. Phys. Rev. B 1981; 24: 1027–1034. DOI: 10.1103/Phys Rev B.24.1027
Lee EH, Hembree DMJr, Rao GR, Mansur LK. Raman scattering from ion-implanted diamond, graphite, and polymers. Phys. Rev. B 1993; 48: 15540–15551. DOI: 10.1103/Phys Rev B.48.15540
Ferrari AC, Robertson J. Interpretation of Raman spectra of disordered and amorphous carbon. Phys. Rev. B 2000; 61: 14095–14107. DOI: 10.1103/Phys Rev B.61.14095
Ferrari AC. Raman spectroscopy of graphene and graphite: Disorder, electron-phonon coupling, doping and nonadiabatic effects. Solid State Commun. 2007; 143: 47–57. DOI: 10.1016/j.ssc.2007.03.052
Morales GM, Schifani P, Ellis G, Ballesteros C, Martinez G, Barbero C, Salavagione HJ. High-quality few layer graphene produced by electrochemical intercalation and microwave-assisted expansion of graphite. Carbon 2011; 49: 2809–2816. DOI: 10.1016/j.carbon.2011.03.008
Petrovski A, Dimitrov A, Grozdanov A, Andonovic B, Paunovic P. Characterization of graphene produced by electrolysis in aqueous electrolytes. In: Petkov P, Tsiulyanu D, Kulisch W, Popov C, editors. Nanoscience Advances in CBRN Agents Detection, Information and Energy Security. NATO Science for Peace and Security Series – A: Chemistry and Biology. The Netherlands: Springer; 2015. p. 103–110. DOI: 10.1007/978-94-017-9697-2_11
Casiraghi C, Ferrari AC, Robertson J. Raman spectroscopy of hydrogenated amorphous carbon. Phys. Rev. B 2005; 72: 085401-1–085401-14. DOI: 10.1103/Phys Rev B.72.085401
Matthews MJ, Pimenta MA, Dresselhaus G, Dresselhaus MS, Endo M. Origin of dispersive effects of the Raman D band in carbon materials. Phys. Rev. B 1999; 59: R6585–R6588. DOI: 10.1103/Phys Rev B.59.R6585
Kavetskyy TS, Tsmots VM, Nowak J, Kuczumow A, Kinomura A, Kobayashi Y, Suzuki R, Mohamed HFM, Šauša O, Nuzhdin V, Valeev V, Stepanov AL. Comprehensive study of carbonization in B+-implanted PMMA: A correlation between slow positron beam and Raman spectroscopy results. In: Proceedings of the 17th International Conference on Positron Annihilation (ICPA‐17); 20–25 September 2015; Wuhan University; Wuhan; 2015. p. 45.
Poly(methyl_methacrylate) [Internet]. 2016. Available from: http://en.wikipedia.org/wiki/Poly(methyl_methacrylate) [accessed 2016-01-28].